Inﬂuence of Carbon Content on Solidifying Shell Growth of Carbon Steels
at the Initial Stage of Solidiﬁcation
and Yuichi Yamaoka2 1
Materials and Processing Research Center, NKK Corp., JFE Fukuyama 721-8510, Japan 2Fukuyama Works, NKK Corp., JFE, Fukuyama 721-8510, Japan
A dipping test that a water cooled copper plate was continuously dipped at 14 mm/s was performed in order to investigate solidifying shell growth in initial solidiﬁcation. Anomalous rough surfaces and uneven shell growth were exhibited for an ultra-low carbon steel (0.005 mass% C) and a hypo-peritectic carbon steel (0.116 mass% C), while for a low carbon steel (0.044 mass% C) and a hyper-peritectic carbon steel (0.304 mass% C), ﬂat surfaces were formed. The carbon content dependence of the anomalous uneven shell growth can be explained by stress caused by solidiﬁcation shrinkage and=transformation occurring from a fraction solid 0.7, where shell begins to have strength, to 1.0, complete solidiﬁcation state. Besides the analysis shows that decrease of the cooling rate can reduce the stress in the shell generated during the initial solidiﬁcation.
(Received October 10, 2002; Accepted February 24, 2003)
Keywords: surface roughness, initial solidiﬁcation, solidiﬁcation shrinkage,=transformation, uneven shell growth, hypo-peritectic carbon steel, ultra-low carbon steel
Steel shell growth in a continuous casting mold is substantially inﬂuenced by carbon content in steel. Shell deformation occurs as a consequence of shell shrinkage due to thermal contraction and=transformation during initial solidiﬁcation. This deformation induces the surface rough-ness of the shell, resulting in anomalous decrease of heat transfer rate from a shell to a mold, often causing uneven shell growth and surface crack in the shell.1–3)
Matsumiya et al.4) have calculated stress and strain in freely shrinking shell within a continuous casting mold. They showed that the maximum tensile stress was resulted in a 0.14 mass% carbon steel in the brittle temperature range near the melting point, and formation of the thinner shell was mathematically modeled from shell deﬂection caused by the thermal stress formed on cooling and the stress induced by = transformation.
Mizoguchi et al.5) have analyzed quantitatively shell growth at the initial stage of solidiﬁcation coupling with the shell deformation due to thermal stress and showed that the unevenness of shell growth is improved by a mild cooling in a mold.
Mizukamiet al.6)have conducted a dipping test of copper chill with measurement of a surface temperature of solidify-ing shell ussolidify-ing a two-dimensional optical pyrometer. They have found out that undercooling and recalesence phenomena appear for ultra-low carbon, low carbon and middle carbon steels and temperature ﬂuctuation on the shell surface after the recarescence is increased in order, low carbon, ultra-low carbon and middle carbon steels. Hence, they have claimed that the deformation of an initial shell is caused by stress in the shell generated by the temperature ﬂuctuation after the recaresence and leads to the uneven shell growth.
In contrast, Esaka et al.7) have performed a dipping test
using two kinds of chill blocks, a ﬂat and a rough blocks in order to investigate the anomalous unevenness of shell growth of a hypo-peritectic carbon steel and simultaneously measured the cooling curve of the start of solidiﬁcation. They have claimed that a diﬀerence of the unevenness of shell growth between the two chill blocks is caused by the nucleation rate. Furthermore, Kajitaniet al.8) have investi-gated the unevenness of shell growth of the ultra-low carbon steel in comparison with that of a 0.15 mass% C steel with the same dipping test. They have concluded that since the nucleation rate for the ultra-low carbon steel is lower than that for the hypo-peritectic carbon steel, the unevenness of shell growth is more anomalously exhibited. However, they do not explain the reason why a mild cooling in a mold can improve the unevenness of shell growth of the hypo-peritectic carbon steel.
Tomonoet al.9)havein-situ observed meniscus shape of liquid metal by carrying out a bottom pouring test and investigated various factors aﬀecting the surface quality of the shell.
Kudohet al.10)have performed a steel chill block dipping test and investigated the eﬀect of the dipping speed of the chill block on the formation of ripple mark and solidiﬁcation structure of the solidiﬁed shell.
Donget al.11)have measured the free deformation of initial
shells of Fe–C alloys with a molten steel droplet method and showed that a very strong deformation in initial shell demonstrates at pure iron and 0.12 mass% carbon steel.
In this study, we have investigated the eﬀect of carbon content in molten steel on the shell growth and its surface quality and found out the anomalous surface roughness and uneven shell thickness of the ultra-low carbon steel and the hypo-peritectic carbon steel. And formation mechanism of the anomalous uneven shell growth generated in the ultra-low carbon steel and the hypo-peritectic carbon steel were discussed with stress induced in a shell due to solidiﬁcation shrinkage and = transformation occurring during solidiﬁ-cation.
*Present address: Industrial Property Coorporation Center, Tokyo
atmosphere, the chemical composition of molten steel was adjusted and the temperature was controlled to maintain superheat to be at 30, 50 and 90 K within10K. Removing scum ﬂoating on the surface of molten steel, a water cooled copper plate, that faces of the copper plate except one face were coated by alumina castable as shown in Fig.1, was dipped continuously at a speed of 14 mm/s. The copper plate was dipped into approximately 250 mm in depth from the molten steel level and subsequently pulled out. The molten steel crystallized and the shell was formed on the copper plate. Transverse surface depressions, which are called ripple mark, were observed on the surface of solidiﬁed shell contact to the copper plate.
The chemical compositions of molten steels were adjusted as shown in Table 1 and the experimental conditions are listed in the same table.
The solidiﬁed shell was machined into its longitudinal direction and at the central width of the shell, and then the shell thickness was measured. A sample for microscopy was taken from a part of longitudinal cross section of the shell. And it was polished to a mirror level, etched with an aqua-solution saturated with picric acid, and subsequently ob-served with an optical microscope.
In order to investigate the characteristics of ripple marks, pitch, depth and curvature radius were measured using a method as shown in Fig.2. The pitch, Lr, is a distance
between two neighboring depressions. The depth, Dr, is a
distance from a shell surface to a tip of ripple mark exposed
by etching. The curvature radius, Rr, of a ripple mark is
approximately expressed by a radius of a single circle inscribing an outer line in a cross section of the ripple mark by using three points shown in Fig.2. These values are averages of measurements of more than 10 ripple marks. Also the thickness of the shells was measured.
3. Results and Discussion
3.1 Inﬂuence of carbon content on surface quality of solidifying shell
Figure3 shows the outer and inner surfaces of solidiﬁed shells for diﬀerent carbon steels: (a) ultra-low carbon steel (0.005 mass% C), (b) low carbon steel (0.044 mass% C), (c) hypo-peritectic carbon steel (0.116 mass% C), (d) hyper-peritectic carbon steel (0.304 mass% C) and (e) high carbon steel (0.678 mass% C). For an ultra-low carbon steel and a hypo-peritectic carbon steel the rough surfaces are clearly revealed in both outer and inner surfaces of the shells.
In contrast, for a low carbon steel, a hyper-peritectic carbon steel and a high carbon steel ﬂat surfaces are exhibited in the both surfaces in comparison with the above two steels.
3.2 Carbon content dependence of the unevenness of solidifying shell growth
Figure4 shows proﬁles of the shell thickness in the longitudinal cross sections of solidiﬁed shells for the ﬁve steels. The uneven shell thickness is revealed anomalously in the ultra-low carbon steel and the hypo-peritectic carbon steel similar to the surface roughness.
Figure5shows the thickness of solidiﬁed shell vs. distance from the upper tip of solidiﬁed shell for diﬀerent carbon steels. Shells of the ultra-low carbon steel and the hypo-peritectic carbon steel grow more unevenly in comparison with those of other steels. For the hypo-peritectic carbon steel, at the early stage of solidiﬁcation the shell grows unevenly, while for the ultra-low carbon steel the shell grows evenly until around 10 seconds from the start of dipping, but after the time the anomalous uneven shell appears.
In contrast, for the low carbon steel and the high carbon steel the shell grows in ﬂat and the thickness are similar to Fig. 1 Schematic diagram of experimental apparatus for dipping test.
Table 1 Chemical compositions of steels used for the dipping test and experimental conditions.
Chemical C: 0.005, 0.05, 0.12, 0.30, 0.70 Molten
(mass%) Si Mn P S sol. Al
<0:02 0.20 0.01 0.01 0.05–0.10 Superheat (K) 30, 50 and 90
Dipping speed (mm/s) 14
Dipping length (mm) ca. 250 Cooling water ﬂow rate (‘/min) 90
Tip of ripple Mark
that of the ultra-low carbon steel. However, although for the hyper-peritectic carbon steel the shell grows evenly, in thinnest thickness among those steels.
The shell thickness (mm),Ds, is experimentally expressed
byDS¼KS ﬃﬃ t
, here,KS is the solidiﬁcation constant (mm/
min1=2) andtis the solidiﬁcation time (min).
The instantaneousKSwas obtained by reverse calculation
using the data ofDsandtin Fig.5. Also the unevenness of
shell thickness was expressed by the standard deviation of
KS. The average value and standard deviation of KS are
calculated and shown in Figs. 6(a) and (b) against carbon content.
On the other hand, theKS can be given by the following
equation derived from heat transfer analysis under the conditions that temperatures in a mold are kept constant when a pure liquid metal crystallizes.12)
K2 S 4
erf KS 2pﬃﬃﬃ
¼ ðTmTsÞ Cp Hf
whereis the thermal diﬀusivity (m2/s),Cp: the speciﬁc heat
capacity (kJ/kgK), Hf: the latent heat (kJ/kg), Tm: the
melting temperature (K), andTsis the interfacial temperature
(K) between a solidifying shell and a mold.
The KS is calculated substituting the following values of
physical properties into eq. (1):is given by Nishiet al.13) such as0:672105,0:682105 and0:629105m2/s
at 1573 K for an ultra-low carbon steel, a low carbon steel and a medium carbon steel, respectively, andCp¼0:67kJ/kgK, Hf ¼272kJ/kg, Tm is given by the liquidus temperature
calculated from the chemical composition, and a temperature diﬀerence, TmTs, is assumed to be 200 K, because the
surface temperature of a shell in a continuous casting mold is predicted about 1573 K. The calculatedKSis around 18 mm/
min1=2and is a little decreased with carbon content. In contrast, when the unevenness of the shell thickness is expressed by the standard deviation of the shell thickness, the unevenness reveals two peaks at the ultra-low carbon steel and the hypo-peritectic carbon steel as shown in Fig.6(a). Fig. 3 Appearance of outer and inner surfaces of the solidiﬁed shells [(a) ultra low carbon steel (0.005 mass% C), (b) low carbon steel
3.3 Characteristics of Ripple Mark
Tomonoet al.9)have studied the shape of meniscus in the solidifying steel shells containing 0.18 to 0.22 mass% carbon with a bottom pouring casting test. The meniscus shape was observed through a silica glass putting into a part of mold when a liquid metal level is rising up and passing through the glass. Fifteen pictures of the meniscus shape were totally taken at ﬁve pictures every second, and the averaged curvature was determined using the pictures. And they examined the pitch, the depth of the ripple mark formed on the ingot.
We measured the pitch, the depth and the curvature radius of the ripple marks similarly and compared them with the Tomono’s observation measured at an upward speed of 8 and 12 mm/s and diﬀerent atmospheres such as air, hydrogen and argon gas.
3.3.1 Pitch of ripple mark
Solidiﬁcation structures of the shells for the ultra-low carbon steel and the hypo-peritectic carbon steel are shown in Fig.7. Arrows in this ﬁgure show the ripple marks.
Figure8shows the relationship between the pitch of ripple mark and the carbon content in solidifying shell. For comparison, Tomono’s data measured under the air atmo-sphere and a copper chill was plotted in this ﬁgure.
Fig. 4 Shell thickness proﬁles in the longitudinal cross section along the dipping direction [(a) ultra low carbon steel (0.005 mass% C), (b) low carbon steel (0.044 mass% C), (c) hypo-peritectic carbon steel (0.116 mass% C), (d) hyper-peritectic carbon steel (0.304 mass% C) and (e) high carbon steel (0.678 mass% C)].
0 5 10 15
0 50 100 150 200 250 300 0.005mass%C
Distance from Upper Tip of Shell (mm)
5 10 15 20
Solidification Time, t/s
Fig. 5 The shell thickness in the dipping direction for various carbon steels.
Fig. 6 Inﬂuence of carbon content on the unevenness of shell thickness and the solidiﬁcation constant,KS.
3.3.2 Depth of ripple mark
Figure9 shows the relationship between the depth of ripple mark and the carbon content in solidifying shell when the superheat ranged from 45 to 55 K. The ultra-low carbon steel and the hypo-peritectic carbon steel have anomalously deeper ripple marks than those of other carbon steels.
The data measured by Tomonoet al.using a copper chill in air is smaller than our observations.
The depth of ripple mark is remarkably aﬀected by superheat in molten steel during dipping test. Figure10 demonstrates the inﬂuence of superheat on the depth of ripple mark for the ultra-low carbon steel. Clearly the higher superheat forms the shallower ripple mark.
3.3.3 Shape of ripple mark
The curvature radius of ripple mark was independent of the carbon content in this study. The curvature radius is shown in Fig.11against the depth of ripple mark.
It is thought that the shape of ripple mark expresses a meniscus form of molten steel level. Tomono et al.9) have showed that the shape of meniscus can be estimated
accurately by the following equation. The shape of any liquid cylinder in mechanical equilibrium, i.e., where the inner pressure (¼gy) is balanced by capillarity pressure (¼S=Rr) can be theoretically determined from12)
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2a2y2 p
where, ais the capillary constant [a¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ2S=g
],S is the
surface energy (N/m) of molten steel,gis the acceleration of gravity andis the density (kg/m3) of molten steel.
In order to investigate the eﬀect of surface energy on the meniscus shape, the surface energies of these steels are given by 1.456 N/m15) and 0.994 N/m16) for the ultra-low carbon steel and a high sulfur (0.1 mass%) low carbon steel, respectively, and the meniscus shape was calculated with eq. (2). The calculated meniscus shapes of those steels are shown in Fig.12. For the case of the high sulfur steel, the calculated shape is diﬀerent from that of the ultra-low carbon
Pitch of Dipple Mark,
0 0.2 0.4 0.6 0.8
Carbon Content (mass%)
∆T(K) S(%) 30 50 50 90
0.01 0.01 0.30 0.01 Tomono et al.8)
Fig. 8 Relationship between pitch of ripple mark and carbon content.
Carbon Content (mass%)
Depth of Ripple Mark,
0 0.2 0.4 0.6 0.8 1.0
This study (∆T=45~55K) Tomono et al.8)
Fig. 9 Relationship between depth of ripple mark and carbon content.
Fig. 10 Inﬂuence of superheat on the depth of ripple mark for ultra-low carbon steel shell.
30 50 90
Radius of Curvature,
0 1 2 3
Depth of Ripple Mark, Dr/ mm Calc. from eq.(2)
steel. However, since there is a very small dependence of carbon content on the surface energy, the curvature radii for diﬀerent carbon steels are nearly equal one another.
The curvature radius was approximately determined by a radius of a single circle inscribing three points on the calculated line of meniscus shape: a points contacting a chill, a point, e.g. 0.5 mm, corresponding to a depth of a ripple mark and a mid-point between the two points. In Fig.11a dotted line shows the relation between calculated curvature radii and the depth of ripple mark calculated from eq. (2).
3.4 Solidiﬁcation in meniscus zone
Solidiﬁcation in the meniscus is calculated with a simple model as shown in Fig. 13. The eﬀect of the shape of meniscus on the solidiﬁcation was replaced by changing thermal resistance. The calculation area was selected as same as one in Fig. 12. In this model, boundary conditions are assumed that the heat energy is extracted from only the copper plate, and is not extracted at the molten steel level and at a distance of 10 mm from the molten steel level.
Next, the shape of meniscus is given by the calculated one in Fig.12(a), and the heat ﬂuxes between a copper plate wall and a solidifying shell were given as shown in Fig.13(b). The heat ﬂuxes, QM0, in contact zone where a molten steel
contacts to the copper plate, andQMx, in meniscus zone, the
molten steel separating from the copper plate, is given by
QMx¼ ½1=ð1=h0þdM=GÞ T ð4Þ
where,h0is the overall heat transfer coeﬃcient [W/(m2(K)]
in the contact zone, T ð¼TMTSÞ: the temperature
diﬀerence (K) between molten steel in the meniscus and contact zones and the copper plate,dM: the thickness (m) of a
gap between a copper plate and a solidifying shell, andGis
the thermal conductivity [W/(mK)] of the air, which was
given by 0.0573 W/(mK) at 1073 K.
The above thermal boundary conditions are summarized in Fig.13(b).
The heat ﬂux in the zone where a shell contacts a copper plate wall was adjusted to meet the calculated shell thickness for a solidiﬁcation time of 0.2 s to form one ripple mark to the observed shell thickness at a superheat of 30 K. The heat ﬂux,
QM0, in the contact zone was given to be4:823106W/m2.
The calculated shell thickness in the meniscus zone is shown in Fig.14 for a superheat of 30 K and 50 K. The meniscus shape was given by that in Fig.12(a). The higher superheat can form the shallower ripple mark.
Fig. 12 Inﬂuence of interfacial energy on the calculated meniscus shape of molten steel [(a)S¼1:5N/m and (b)S¼0:9N/m].
Fig. 13 Analytical model of solidiﬁcation in the meniscus zone.
0 2 3 4 5
Meniscus shape for an ultra-low C steel calculated from eq.(2)
3.5 Strain induced in a shell caused by solidiﬁcation shrinkage and = transformation during solidiﬁcation
In order to estimate strain induced in a solidifying shell in the initial solidiﬁcation, the rate, RSol, of solidiﬁcation
shrinkage and the rate, R=, of = transformation were
The microsegregation and the= transformation during solidiﬁcation of Fe–C alloys were calculated with a model as shown in Fig.15similar to that made by Ueshimaet al.17) The R= is governed by diﬀusion of carbon in -iron and
-iron in an interdendritic region.
@C=@t¼Di@2C=@x2 ði¼ or -ironÞ ð5Þ
t¼0; C¼C0 ð6Þ
t>0; C=C‘¼k=‘ at x¼x=‘ ð7aÞ
C=C ¼k= at x¼x= ð7bÞ
t>0; @C=@x¼0 at x¼0 and d1 ð8Þ
whereCis the carbon content (mass%),C0: the initial carbon
content (mass%), Di: the diﬀusion coeﬃcient (mm2/s) of
carbon in iron of phase i, k=‘ andk=: the equilibrium of
partition ratios (-) of carbon at the=‘and=interfaces,d1:
the primary dendrite arm spacing (mm),x: the distance (mm) from a reference point in a half of d1, x=‘ and x=, the
distance (mm) between the=‘ interface at the start of the peritectic reaction and the =‘ and the = interfaces, respectively, andtis the diﬀusion time (s).
Equation (5) was solved by a ﬁnite diﬀerence approxima-tion under initial and boundary condiapproxima-tions [eqs. (6)–(8)]. In this study,d1was given by 0.2 mm, which is a primary arm
spacing of dendrite near a surface in continuously cast slab,
and the interdendritic region was divided into 50 elements. Time increment,t, is taken to be 0.00001 s. The equilibrium partition ratios and diﬀusion coeﬃcients are in the litera-ture.17)Since perfect mixing is assumed in liquid phase, the carbon content is uniform.
The ﬂow chart of calculation is shown in Fig. 16. First, the temperature, T, in the interdendritic region is given by a cooling curve and compared with the liquidus temperature,
TL, given by chemical composition of the liquid phase. When
theTis lower than theTLand the carbon content in the liquid
phase is smaller than the carbon content (Ceu) at which the
crystallization of-iron begins to occur, -iron crystallizes. The carbon atom is distributed into -iron and liquid steel phases assuming equilibrium solidiﬁcation.
Second, when the carbon content (CL) in liquid phase
reaches theCeu, the peritectic reaction begins to occur. Just
after the start of peritectic reaction when the-iron crystal-lization and the=transformation take place simultaneous-ly, the carbon content (C) in a mesh of solidiﬁed-iron in
the nearest neighborhood of the /liquid steel interface is determined to make the ratio of carbon content in the meshes on both sides of the /liquid steel interface equal to the equilibrium partition ratio. Also, the=interface shifts one mesh to-iron phase side and-iron phase is extended when the ratio of carbon content in a-iron mesh to that in a-iron mesh at the= interface becomes equal to the equilibrium partition ratio.
δ-iron phase γ-iron phase Liquid phase
j=1 n1n1+1 n2 n2+1 j=n3 diffusion
δ/γ Interface Solid/Liquid Interface
1 C k
C2/ C2+1= γ d1
Fig. 15 Calculation model for formation of microsegregation and = transformation on cooling.
δ/γ transformation in solid
δ/γ transformation or not
γ−crystallization or not
Diffusion in solid
t < tend
end T < Tliq
CL< Ceu T → T-CR×t
Diffusion in solid no
no yes t → t+∆t
mode is changed to-iron crystallization mode, and the -iron crystallizes.
Shinet al.18)conducted a hot tensile test and deformed a
test piece to a failure after being melted and then solidiﬁed in a testing machine. They showed that the tensile strength begins to arise in a fraction solid of 0.6 to 0.7.
At the initial stage of solidiﬁcation the shell strength is too low, and hence the shell is easy to be deformed by thermal stress and=transformation stress. In this study, in the case of peritectic reaction formed during solidiﬁcation, the volume,Vtr, and the rate,Rtr, of transformation include both
the solidiﬁcation and the=transformation formed during a fraction solid of 0.7 to 1.0. On the other hand, in the case of no peritectic reaction, the Vtr and the Rtr include only
Two cooling rate was selected, 5 K/s and 0.5 K/s. A cooling rate of 5 K/s corresponds to that at a slab surface in a continuous casting mold and a cooling rate of 0.5 K/s is assumed as an example of extremely mild cooling.
The calculated volume and rate,Rtr, at a cooling rate of 5
and 0.5 K/s are plotted in Fig.17against carbon content. The calculated volume is normalized by dividing an initial volume and expressed by Vtr=V0. The Vtr=V0 is remained
constant before initiation of = transformation and after completion of=transformation as shown in Fig.17(a). And it increases with carbon content of 0.08 to 0.18 mass% C,
low carbon steel and the hypo-peritectic carbon steel, and has a minimum in approximately 0.04 mass% C. Furthermore, the rate is extremely decreased by decreasing cooling rate. Also, theRtris decreased with decreasing cooling rate.
A stress-strain relation at elevated temperatures is given by19)
¼F"n""_mexpðQ=RTÞ ð9Þ whereis the stress (MPa),": the strain (-),""_: the strain rate (s1),n: the strain exponent (-),m: the strain rate exponent (-),Q: the activation energy (J/mol),R: the gas constant andT
is the temperature (K).
The strain generated in a shell during solidiﬁcation is expressed as "solþ"=, where "sol is the strain due to the
solidiﬁcation shrinkage and "= is the strain due to =
transformation, and the "solþ"= is related to a volume
change caused by transformation. The strain rate is assumed to be an average during a fraction solid of 0.7 to 1.0, and corresponds to a sum of the rates of the solidiﬁcation and the = transformation. A product between the transformation volume and the transformation rate is corresponding to a stress expressed by eq. (9). In this study, a product between the transformation volume and the transformation rate is given byðVtr=V0Þ Rtr, which is called stress index. The stress
index vs. carbon content is shown in Fig.18 for diﬀerent cooling rate, exhibiting two peaks in the ultra-low carbon steel and the hypo-peritectic carbon steel and decreasing with decreasing cooling rate.
Consequently, the = transformation occurring during solidiﬁcation in the higher fraction solid is conﬁrmed to lead to the greater shell deformation and the larger air gap, resulting in an uneven shell growth with some deﬂection and anomalous reduction of heat ﬂux in a mold, which in turn causes local recalescence of the deﬂected portion of the shell to reduce the shell strength.
The analytical results such that the stress induced in a shell
Fig. 17 Inﬂuence of carbon content on the calculated rate and volume of solidiﬁcation and=transformation occurring in a solid fraction 0.7 to 1.0.
is reduced by a mild cooling gives the understanding of the reason for the eﬀect of the mild cooling in a mold on the prevention of longitudinal surface crack in the hypo-peritectic carbon steel.
A dipping test using a copper plate cooled by water was performed to quantitatively investigate the inﬂuence of carbon content in solidifying steel on shell growth.
Anomaly in the unevenness of shell thickness and the depth of ripple mark was revealed for an ultra-low carbon steel and a hypo-peritectic carbon steel. Increase of the superheat in molten steel can reduce the depth of ripple mark. Furthermore, analysis of solidiﬁcation of Fe–C alloys accompanying with= transformation was made to clarify the shell deformation resulting in the anomaly in surface roughness and shell thickness unevenness of solidifying shells for the ultra-low carbon steel and the hypo-peritectic carbon steel.
The carbon content dependence of the calculated stress index is in good agreement with the observed one of the uneven shell growth. The product between the volume and the rate of the solidiﬁcation shrinkage and the = transfor-mation formed until crystallization is completed after a shell begins to have a strength and,i.e., during a fraction sold of 0.7 to 1.0, exhibits two peaks for the ultra-low carbon steel and the hypo-peritectic carbon steel. Besides the analysis shows that a mild cooling in a mold can reduce the stress generation.
1) A. Grill and K. Brimacombe: Ironmak. Steel.3(1976) 76–79. 2) S. N. Singh and K. E. Blazek: Open Hearth Proc. AIME59(1976) 264–
3) T. Saeki, S. Oguchi, S. Mizoguchi, T. Yamamoto, H. Misumi and S. Tuneoka: Tetsu-to-Hagane´68(1982) 1773–1781.
4) T. Matsumiya, T. Saeki, J. Tanaka and T. Ariyoshi: Tetsu-to-Hagane´68
5) T. Mizoguchi, S. Ogibayashi and T. Kajitani: Tetsu-to-Hagane´ 81
6) H. Mizukami, S. Hiraki, M. Kawamoto and T. Watanabe: ISIJ Int.39
7) H. Esaka, T. Shirakami, T. Mizoguchi and S. Ogibayashi: Tetsu-to-Hagane´81(1995) 631–636.
8) T. Kajitani, H. Esaka, M. Wakoh, H. Misumi and S. Ogibayashi: Tetsu-to-Hagane´81(1995) 1055–1060.
9) H. Tonomo, W. Kurz and W. Heinemann: Metall. Trans.12B(1981) 409–411.
10) M. Kudoh, T. Takahashi and Y. Deguchi: Tetsu-to-Hagane´73(1987) S901.
11) S. Dong, E. Niyama and K. Anzai: ISIJ Int.35(1995) 730–736. 12) D. P. Poirier and G. H. Geiger:Transport Phenomena in Metallurgy,
(TMS, 1994), 337.
13) T. Nishi, H. Shibata, K. Tsutsumi, H. Ohta and Y. Waseda: ISIJ Int.42
14) J. J. Berkerman:Physical Surfaces, (Academic Press, London,1970) p. 12.
15) Handbook of Physical Properties of Molten Steels and Molten Fluxes, (ISIJ, 1972) p. 124.
16) Handbook of Physical Properties of Molten Steels and Molten Fluxes, (ISIJ, 1972) p. 128.
17) Y. Ueshima, S. Mizoguchi, T. Matsumiya and H. Kajioka: Metall. Trans.17B(1986) 845–859.
18) K. Shin, T. Kajitani, T. Suzuki and T. Umeda: Tesu-to Hagane´78